Ammonia Stress Corrosion Cracking
mmonia Stress Corrosion Cracking (SCC) is the phenomena of cracks being formed in carbon steel in contact with ammonia. The cracks are small at the surface but can be deep, worstcase going through the entire thickness of the metal. See photo below.
the problem with SCC
SCC can threaten the integrity of the ammonia containment equipment. Stress Corrosion Cracking has been detected in ammonia storage tanks, spheres and other process equipment that is in contact with liquid ammonia. It can happen at atmospheric liquid ammonia conditions at -33 째C, but also at higher temperatures under pressurized ammonia conditions. Also tanks for transporting liquid ammonia, like rail tank cars, tank cars, barges and vessels can be susceptible to stress corrosion cracking. It is difficult to repair SCC damage. Often complete replacement of the equipment (like a new tank) is necessary when SCC is found.
the root cause for this SCC
The presence of oxygen (air) and residual stress are the causes for forming SCC cracks. Therefore the ingress of air into ammonia containing equipment must be prevented. This is a shared responsibility of the ammonia producing and consuming industries. Through the transport of ammonia via rail tank cars, barges or vessels, oxygen can be transported from one location to the other. Also the return of empty transport tanks can be a source of oxygen.
can we prevent SCC
Make sure not to have oxygen (air) present. Typical sources of oxygen are hoses, (un)loading pipe work, process equipment that has been open (after a turnaround or an inspection), vacuum conditions. One should apply nitrogen purging systems to prevent air getting into the ammonia system, and only when all air is out one should take in operation ammonia equipment that has been opened. And also be sure that your supplier or customer is not â€œpolluting the ammonia transportation chainâ€? with oxygen. Regular system analysis on the oxygen content can assure the absence of oxygen.
Add at least 0.2 % water to the ammonia. Water prevents the formation of SCC cracks. This measure does not mean that one should not try to still minimise oxygen ingress.
or Apply stainless steel equipment. Stainless steel is not susceptible to SCC. But be aware that when you operate using stainless steel equipment with high oxygen levels, you may pass the problem on to others in the ammonia chain. When carbon steel is used, post weld heat treatment must be performed to reduce residual stresses. Weld hardness should not exceed 225 HV.
Avenue E. van Nieuwenhuyse 4/6 B-1160, Brussels, Belgium Tel: +32 2 675 3550 Fax: +32 2 675 3961 firstname.lastname@example.org
www.productstewardship.eu www.fertilizerseurope.com twitter.com/FertilizersEuro
For methods on how to analyse for oxygen in ammonia see appendix 4 in the Guidance document for Inspection of Atmospheric Refrigerated Ammonia Storage Tanks (2008) at www.fertilizerseurope.com
Stress Corrosion Cracking